Zone Axis

Get Zone Axis essential facts below. View Videos or join the Zone Axis discussion. Add Zone Axis to your PopFlock.com topic list for future reference or share this resource on social media.

## Zone-axis indexing

## Zone-axis patterns

## See also

## Footnotes

## External links

This article uses material from the Wikipedia page available here. It is released under the Creative Commons Attribution-Share-Alike License 3.0.

Zone Axis

This article may be too technical for most readers to understand. Please to make it understandable to non-experts, without removing the technical details. (October 2014) (Learn how and when to remove this template message) |

**Zone axis**, a term sometimes used to refer to "high-symmetry" orientations in a crystal, most generally refers to *any* direction referenced to the direct lattice (as distinct from the reciprocal lattice) of a crystal in three dimensions. It is therefore indexed with direct lattice indices, instead of with Miller indices.

High-symmetry zone axes through a crystal lattice, in particular, often lie in the direction of tunnels through the crystal between planes of atoms. This is because, as we see below, such zone axis directions generally lie within more than one plane of atoms in the crystal.

Crystal-lattice translational invariance^{[1]}^{[2]} is described by a set of unit-cell direct-lattice (contra-variant^{[3]} or polar) basis-vectors **a**, **b**, **c**, or in essence by the magnitudes of these vectors (the **lattice parameters** a, b and c) and the angles between them (namely α between **b** and **c**, β between **c** and **a**, and γ between **a** and **b**). Direct-lattice vectors have components measured in distance units, like meters or angstroms.

These lattice vectors are *indexed* by listing one (often integral) multiplier for each basis-triplet component, generally to be placed between either square [] or angle ⟨⟩ brackets. Thus the direct lattice-vector **s**_{uvw} or [u,v,w] is defined as u**a**+v**b**+w**c**. Angle brackets are used when you don't want to refer to a specific lattice vector, but to a symmetrically equivalent class of lattice vectors. In the case of a cubic lattice, for instance, ⟨100⟩ represents [100], [010] and [001] because each of these vectors is symmetrically equivalent.

The term zone axis, more specifically, refers to only the *direction* of a direct-space lattice vector. For example, since the [120] and [240] lattice vectors share a common direction, their orientations *both* correspond the [120] zone of the crystal. Just as **a set of lattice-planes in direct-space corresponds to a reciprocal-lattice vector** in the complementary-space of spatial-frequencies and momenta, a "zone" is defined^{[4]}^{[5]} as **a set of reciprocal-lattice planes in frequency-space that corresponds to a lattice-vector** in direct-space.

The reciprocal-space analog to zone axis is "lattice-plane normal" or "g-vector direction". Reciprocal-lattice (one-form^{[6]} or axial) vectors are *Miller-indexed* using the reciprocal-lattice basis-triplet (**a***, **b***, **c***) instead, generally between either round or curly {} brackets. Curly brackets are used when you don't want to refer to a specific reciprocal-lattice vector, but to a symmetrically equivalent class of reciprocal-lattice vectors.

Here as usual **a*** ≡ **b**×**c**/V_{c}, **b*** ≡ **c**×**a**/V_{c}, and **c*** ≡ **a**×**b**/V_{c}, where the unit cell volume is V_{c} = **a**•(**b**×**c**). Thus reciprocal-lattice vector **g**_{hkl} or (h,k,l) = h**a***+k**b***+l**c*** has a direction perpendicular to the (hkl) crystallographic plane, and a magnitude g_{hkl} = 1/d_{hkl} equal to the reciprocal of the spacing between (hkl) planes, measured in spatial-frequency units e.g. of cycles per angstrom.

Object | Generic Type | Specific Instance | Units | Transformation |
---|---|---|---|---|

zone or lattice-vector s_{uvw} |
direct space e.g. [meters] | contra-variant or polar | ||

plane or g-vector g_{hkl} |
reciprocal space e.g. [cycles/m] | co-variant or axial |

A useful and quite general rule of crystallographic "dual vector spaces in 3D" is that the condition for a direct lattice-vector [uvw] to have a direction (or zone-axis) perpendicular to the reciprocal lattice-vector [hkl] is simply hu+kv+lw = 0. This is true even if, as is often the case, the basis-vector set used to describe the lattice is not Cartesian.

By extension, then, a [uvw] **zone-axis pattern** (ZAP) is a diffraction pattern taken with an incident beam e.g. of electrons, X-rays or neutrons traveling along a lattice direction specified by the zone-axis indices [uvw]. Because of their small wavelength λ, the high energy electrons used in electron microscopes^{[7]} have a very large Ewald sphere radius (1/λ) so that electron diffraction generally "lights up" diffraction spots with g-vectors (hkl) that are perpendicular to [uvw], i.e. for which hu+kv+lw=0.

One result of this, as illustrated in the figure above, is that "low-index" zones are generally perpendicular to "low Miller-index" lattice planes, which in turn have small spatial frequencies (g-values) and hence large lattice periodicities (d-spacings). Put another way, in electron microscopy^{[8]}^{[9]}^{[10]}^{[11]} if you want your electron beam to be directed down wide (hence easily visible) tunnels between columns of atoms in a crystal, directing the beam down a low-index (and by association high-symmetry) zone axis may help to this end.

- Crystallography
- Dual basis
- Reciprocal lattice
- Miller index
- Diffraction
- Electron diffraction
- Transmission electron microscopy

**^**J. M. Ziman (1972 2nd ed)*Principles of the theory of solids*(Cambridge U. Press, Cambridge UK).**^**Zbigniew Dauter and Mariusz Jaskolski (2010) "How to read (and understand) Volume A of International Tables for Crystallography: an introduction for nonspecialists",*J. Appl. Cryst.***43**, 1150-1171 pdf**^**George Arfken (1970)*Mathematical methods for physicists*(Academic Press, New York).**^**E. W. Nuffield (1966)*X-ray diffraction methods*(John Wiley, NY).**^**B. E. Warren (1969)*X-ray diffraction*(Addison-Wesley, paperback edition by Dover Books 1990) ISBN 0-486-66317-5.**^**cf. Charles W. Misner, Kip S. Thorne and John Archibald Wheeler (1973)*Gravitation*(W. H. Freeman, San Francisco CA).**^**John M. Cowley (1975)*Diffraction Physics*(North-Holland, Amsterdam).**^**P. Hirsch, A. Howie, R. Nicholson, D. W. Pashley and M. J. Whelan (1965/1977)*Electron microscopy of thin crystals*(Butterworths/Krieger, London/Malabar FL) ISBN 0-88275-376-2**^**J. W. Edington (1976)*Practical electron microscopy in materials science*(N. V. Philips' Gloeilampenfabrieken, Eindhoven) ISBN 1-878907-35-2**^**Ludwig Reimer (1997 4th ed)*Transmission electron microscopy: Physics of image formation and microanalysis*(Springer, Berlin) preview.**^**David B. Williams and C. Barry Carter (1996)*Transmission electron microscopy: A textbook for materials science*(Plenum Press, NY) ISBN 0-306-45324-X

This article uses material from the Wikipedia page available here. It is released under the Creative Commons Attribution-Share-Alike License 3.0.

Popular Products

Music Scenes

Popular Artists